Thermodynamically-consistent phase-field models for solidification

Thermodynamically-consistent phase-field models for solidification

Physica D 69 (1993) 189-200 North-Holland SDI- 0167-2789(93)E0226-2 Thermodynamically-consistent phase-field models for solidification S.-L. W a n g ...

Physica D 69 (1993) 189-200 North-Holland SDI- 0167-2789(93)E0226-2

Thermodynamically-consistent phase-field models for solidification S.-L. W a n g a, R . F . S e k e r k a a'1, A . A . W h e e l e r b, B . T . M u r r a y c, S . R . C o r i e l l c, R.J. Braun ~ and G.B. McFadden ¢ "Department of Physics, Carnegie Mellon University, Pittsburgh, PA 15213, USA bSchool of Mathematics, University of Bristol, Bristol BS8 1 TW, UK CNational Institute of Standards and Technology,: Gaithersburg, MD 20899, USA

In an effort to unify the various phase-field models that have been used to study solidification, we have developed a class of phase-field models for crystallizationof a pure substance from its melt. These models are based on an entropy functional, as in the treatment of Penrose and Fife, and are therefore thermodynamically consistent inasmuch as they guarantee spatially local positive entropy production. General conditions are developed to ensure that the phase field takes on constant values in the bulk phases. Specificforms of a phase-field function are chosen to produce two models that bear strong resemblances to the models proposed by Langer and Kobayashi. Our models contain additional nonlinear functions of the phase field that are necessary to guarantee thermodynamic consistency.

1. Introduction

T h e classical approach to the modeling of first order phase transformations involves tracking of the free boundary that separates the growing phase from the parent phase. This requires the solution of a formidable free boundary problem. For example, for crystalization of a solid (crystal) from a pure liquid (melt), one must solve the equations for the temperature fields in both solid and liquid subject to boundary conditions for the temperature and its derivatives on the moving solid-liquid interface, the free boundary. The phase-field model provides an alternative approach, according to which a new variable, the phase field ~b, is introduced to keep track of the phase, taking on constant values indicative of each of the bulk phases and making a transition

1Consultant, National Institute of Standards and Technology. ~Teehnology Administration, US Department of Commerce, Washington, DC.

between these values over a thin transition layer that plays the role of the classically sharp interface. The phase field ~b is governed by a partial differential equation that guarantees (in the asymptotic limit of a suitably thin transition layer) that the appropriate boundary conditions at the crystal-melt interface are satisfied. Moreover, the transport equations are modified, by addition of terms that depend on the phase field, to apply in all of space and to e m b o d y the conservation conditions at the interface. One then proceeds to solve the coupled equations for the phase field and transport-related fields (e.g., temperature a n d / o r composition) without the necessity of explicit tracking of the free boundary. Langer [1,2] adapted Model C of Halperin, Hohenberg and Ma [3] to produce a phase-field model that accounts for the G i b b s - T h o m s o n equation at the solid-liquid interface for solidification problems. Moreover, a similar phase-field model was introduced by Collins and Levine [4]. Analytical properties of the phase-field equations

190

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

resulting from Langer's model have been analyzed extensively by Caginalp et al. [5-13], Gurtin [14] and Fife and Gill [15,16]. In particular, Caginalp [11] has shown that certain distinguished limits of the phase-field equations lead to various free boundary problems, including the classical models of solidification. Numerical methods for computation using a phase-field model were introduced by Fix [17] and early numerical computations in one dimension were performed by Lin [18]. Subsequently, there have been a number of computations in one dimension, including those by Schofield and Oxtoby [19] for planar geometries and by Caginalp and Socolovsky [12] for planar and spherically symmetric geometries. Success with numerical computations for more complex shapes has been limited because of the considerable computational power needed to resolve the diverse length and time scales intrinsic to the phase-field model. Recently, Kobayashi [20] introduced a phase-field model that he used to compute the dendritic solidification of a pure material from a supercooled melt, in two [21,22] and three [23] dimensions. Using the phase-field model described in the present paper, numerical computations in two dimensions have been carried out for the dendritic growth of nickel by Wheeler et al. [24]. In all computations of dendritic growth based on phase-field models, it has so far been necessary to employ high undercoolings in order to mitigate the disparity of the thermal length scale and the interface thickness. A difficulty with phase-field models, as pointed out by Penrose and Fife [25], lies in their derivation. In particular, the governing equation for the phase field is usually derived from a free energy functional that is applicable only to an isothermal situation; then the classical equation for the temperature field is altered in an ad hoc manner to account for the liberation of latent heat by addition of a term proportional to the time derivative of the phase field. Penrose and Fife, however, provided a framework from which the equations for the phase field and the

temperature can be derived in a thermodynamically consistent manner from a single entropy functional. In the present paper, we employ the method of Penrose and Fife to derive a class of phasefield models for the crystallization of a pure material from its melt that have the following properties: (1) They are based on an entropy functional and guarantee local positive entropy production, (2) The functions and parameters in the model can be chosen to agree with empirical data, such as heat capacity per unit volume and surface tension, asymptotically in the classical limit, (3) They satisfy criteria to ensure that the phase field will take on fixed values, which we take to be 0 for the solid and 1 for the liquid, for the bulk phases, (4) They allow for specific choices of the phase-field function that lead to models, which we call Model I and Model II, that bear a strong resemblance to the models of Langer and Kobayashi, respectively, but that display specific nonlinearities necessary to satisfy properties (1)(3). Thus, we provide a common basis for their models.

2. Thermodynamic formulation For purposes of deriving the partial differential equations for the phase-field model, we consider a closed system of volume V in which a pure material undergoes a first-order phase transition between solid and liquid. We introduce an order parameter ~b(x, t), called the phase field, that indicates the phase of the material at (x, t). We assume that ~b equals zero in the solid phase and unity in the liquid phase. Thin regions, in which th takes values between zero and unity, will be shown to correspond to crystalmelt interfaces. For simplicity, we assume uni-

S.-L. Wanget al. / Thermodynamically-consistentphase-fieldmodelsfor solidification form density throughout the system and that there is no convection in the liquid; this ensures mechanical equilibrium. We assume that the internal energy of any subvolume ~ of V is represented by the integral

v(0s3

0s

*q+e2~V~b

--

191

]

°

nda

,

(5b)

~t

= f e dr.

(1)

According to the first law of thermodynamics, the time rate of change of ~ obeys

¢g + f q . n d a = O ,

(2)

#+

~t

where M is the surface of o//. with outward normal n, and q is flux of internal energy. Converting the surface integral in eq. (2) to a volume integral by Gauss' theorem and equating the integrands, which is permissible since ~ is arbitrary, leads to the familiar equation + V. q = 0.

(3)

The entropy of any subvolume ~ of V is assumed to be represented by the functional 6e =

f Is- ½e2(V~b)2] dv,

t\ael,

da->0,

(6)

where T is the absolute temperature. In eq. (6), q/T is the familiar entropy flux due to heat flow; the quantity ~2~Vtk is an entropy flux related to changes in the phase field at the boundary of the subvolume ~. The volumetric entropy production and the entropy flux associated with ~b will be related to their counterparts for a sharpinterface model in the discussion section. Substitution of eq. (5b) into eq. (6) then leads to

(4)

where s(e, ¢~) is an entropy density (an extension of classical thermodynamics) that would apply to a uniform system of internal energy density e and phase field ~b, a n d ~ is a constant. The second term in the integrand is a gradient entropy term analogous to the Landau-Ginzburg or CahnHilliard gradient energy term in the free energy, cf. eq. (37). Differentiation of eq. (4) with respect to time gives

#=f

where we have substituted for ~ from eq. (3) and used Gauss' theorem to integrate by parts. The second law of thermodynamics requires the entropy production to be positive in any subvolume ~ of V. This entropy production can be calculated by subtracting from ~ the entropy flux through M, which leads to the relation

where we have used de = T ds +

d~

(8)

\$

to identify (Os/Oe), = ( l / T ) . We can therefore guarantee local positive entropy production by choosing

(1)

q = MrV -~ ,

(9) (10)

+[(-~),+

-E2V • (~V~b)} do

e

(5a)

where M r and r are positive. This choice allows the integrand in eq. (7) to be reduced to a sum

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

192

T

of squares: [ql2/M r +T(~) 2. The governing equations therefore become

f e(¢i?--------~)d, +

(16)

TM

where G(~b) is an undetermined function of ~b and T M is the melting point. To proceed further, we assume that the initial energy density has the form

for the internal energy density, and

~=

_l(0e~

r~a~/, +'2v~6

(12)

= eL(T) +

for the phase field. In order to identify the derivative in eq. (12), it is convenient to work with the Helmholtz free energy density

f=e-

Ts,

[P(4') - IIL(T),

whose differential, when combined with eq. (8), yields

.4,

and

(0[f/rl~

aT /~,

(17)

where es(T ) and eL(T ) are the classical internal energy densities of the solid and liquid phases, respectively, and L(T)= eL(T ) --es(T ) is their difference. Here p(~b) satisfies p ( 0 ) = 0 and p(1) = 1. We note that Lo =- L(TM) is the latent heat of fusion; whereas the variation of L(T) > 0 with temperature allows the heat capacities per unit volume of solid and liquid to depend differently on temperature, as illustrated in fig. 1. From eq. (16), the free energy density corresponding to this internal energy density is

(13)

(0e) (0,)

L(T)

e = es(T) + p ( ¢ )

T

=

f(T,~b)=T(-

e

- T----~.

(15)

f eL(g') TM

-[p(,~) - llQ(T) + G(4,)),

The latter can be integrated at constant ~b to give

(18)

I I I

e

~..- ~

L(TI)

,,~

&

I

I rM

r

Fig. 1. Sketch of the internal energies eL(T ) and es(T ) as functions of temperature. The solid curves correspond to the stable bulk phases, whereas the dashed curves correspond to either supercooled liquid or superheated solid. The difference between the curves at any temperature is the function L(T), which is equal to the latent heat Lo =- L(TM) at the melting point T M.

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

where

1

G(4,) = ~ - g(4'),

T

Q(T)=

193

f -L(~) -~- de.

(19)

(29)

where

TM

We note that Q(T) is monotonic increasing with respect to its argument, T, and Q(TM) = 0. From eq. (14) and eq. (18) we have

O(-yZ) \$ = - T Q ( T ) P'(4') + TG'(4,) .

(20)

Thus, the governing equations, eq. (11) and eq. (12), become OL(T) + :(4') L(T) + [P(4') - 1]L(T)

and

~-~ = Q ( r ) p'(4,) - a'(4,) + ~ v 2 4 , .

(22)

We have assumed that 4' = 0 and 4' = 1 correspond to bulk solid and liquid states for all values of the temperature. This consideration requires f to have, for all values of T, local minima with respect to 4' at 4' = 0 and 4' = 1. We also require f to be continuous with respect to the temperature at the melting point; therefore

f ( T M, 0) = f(TM, 1),

(23)

g(4,) = 4,2( 1 - 4,)Z,

and a is a positive constant; this choice implies the convention f ( T M, 0) = f ( T M, 1) = 0. In the next section we explore two possible choices for P(4') which lead to phase-field models that may be compared to those of Langer and Kobayashi. We continue with the general development of the phase-field equations by further specifying the thermodynamic description of the system. For a pure material, one is mostly interested in studying morphological instabilities and subsequent dendritic growth that can occur in solidification from an undercooled melt, where heat conduction takes place mostly in the liquid. Therefore, in order to obtain a tractable problem, we assume the energy density in the liquid to be a linear function of temperature of the form eL(T ) = eL(TM) + c ( T - TM) ,

(24)

(31)

where c is a constant heat capacity per unit volume, which will lead to the classical heat equation in the bulk liquid. Eq. (21) and eq. (22) therefore become ,

Of 4,=o,1 = 0, 04,

(30)

OT

{c + [P(4') - 1]L (T)) ~

,.

= kV2T,

02f

[

04, 2 ,~o,~

> O.

(25)

G(0) = G ( 1 ) ,

(26)

[G'(4,) - P'(4') Q(T)][• =0,1 = 0,

(27)

[G"(4,) - p"(4,) Q(T)][,.0,, > O.

(28)

Accordingly we choose G(4,) to be a symmetric 'double well' potential with minima at zero and unity of the form

(32)

and 04, 1 , r-~? = Q(T) p'(4,) - ~ g (4,) + ~2v24,,

These conditions require that

04,

+ L(T) p (4,) - ~

(33)

where we have set M r = k T 2. The thermal conductivity k is assumed to be constant. At this point in the development of the equations, the parameters a and e can be related to the interface thickness and surface free energy by examining a one-dimensional solution of eq. (33) under equilibrium conditions, T = T M, for which it becomes

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

194

2 d2~b e dx 2

1 4a g'(~b) = 0,

(34)

with boundary conditions ~b--~0 as x--~-o% and ~b-~ 1 as x--~ + oo. The solution is found to be ~b(x)=-~ tanh 2--~--£e + 1 ,

(35)

where we have chosen a constant of integration to locate the interface at x = 0. From this solution it is clear that the interface has characteristic thickness 8 = x/8 e .

(36)

To calculate the surface free energy associated with the one-dimensional solution, we employ the Helmholtz free energy functional at temperature TM, which from eq. (4) and eq. (1) is given by

x £= ~,

~_

t w2/r

T-

and

TM

u- Tu-T o'

where T O is an appropriate reference temperature, typically taken to characterize the temperature of the external boundary for Dirichlet conditions, or to characterize the initial temperature for Neumann conditions. Here, a tilde is used to denote the dimensionless equivalent of a dimensional quantity. The governing equations become

£'(u) ou

(1 + [p(~b) - 1] ~ ) - - ~

£(u) T p ' ( 6 ) 0t" = V2u,

g2 a 6 _ g27% + m

(40)

s0(u) p'(6) _ 1g,(6)

Ot

(41) ~: = ~ - T~a0°

where

= j [ f ( T M , 4~) + ½e2TM(V6) 2] d r .

(37)

(42)

£(u) = L/L o ,

V

The corresponding surface free energy per unit area, which is a surface excess quantity because f ( T M , ~b)= 0 in the bulk, is

Q(u) = and

i 0

L(~') d~', {1 + [(T M - T o ) / T M ] ¢ } 2

(43)

+do

v2 w[L0]2 o"

M\ d x ]

dx.

(38)

V~STm 12a

12c0.T M

8 ~: = ~

This may be evaluated to yield 0.

a

W '

(39)

Hence, the constant a is related to the material parameters and the interface thickness 8. In order to proceed further, it is advantageous to nondimensionalize the governing equations. We introduce a length scale w representative of the size of the domain, and use the thermal diffusion time w 2 & , where K = k / c is the assumed constant thermal diffusivity of the liquid, as the reference time scale. Employing these scales, we write

rn =

c(rM - r0) ,

S=

6 V ~ 8o" "rK T M

Lo .

, (44)

Below, we determine m explicitly in terms of the interface kinetic coefficient and known material parameters. We shall proceed to discuss eqs. (40)-(44) for two different choices of p(th) given below. 3. Phase-field models I and II

In order to proceed in the development of the phase-field model, the function p(~b) which appears in the energy density must be specified. We consider two different polynomial forms for the

S.-L. Wang et al. / Thermodynamically-consistentphase-field models for solidification

function p(tb) which result in different phasefield models. M o d e l I. We choose

~ g(sr) g(~') d~" d~" - ~b3(10_ 15~b + 6~b2) P(4~) - fj.~

(45)

which satisfies the required normalization that p(0) = 0 and p ( 1 ) = 1 as well as the conditions eq. (27) and eq. (28), independent of Q ( T ) , because p'(~b)=p"(~b)--0 at ~b = 0 and 1. This choice will lead to a phase-field model that we will compare with the one proposed by Langer [2]. Model H. We choose

3.1. M o d e l I

Eq. (45) applies and there are no restrictions on Q ( T ) . Therefore, for simplicity, we choose the heat capacity per unit volume of the solid to equal the constant heat capacity per unit volume, c, of the liquid, in which L ( T ) = Lo, which results in £(u)-= 1. We also assume that ITM 7"ol ~ T M and so we make the approximation Q(u) = u. Thus, eq. (40) and eq. (41) become 30g(\$) O~b -zS Ot

V2u

'

(47)

-2

04~ = - g2vz~b + 30g(~b) gaSu - lg'(~b) m Ot

E

Ou ---z = V2u Ot

(49)

(46)

which satisfies the conditions that p ( 0 ) = 0 and p ( 1 ) = 1, and p'(0) = p'(1) = 0; however, because G"(0) - p"(O) Q ( T ) -= 1/2a - 6Q(T) and G"(1) - p ' ( 1 ) Q ( T ) = 1/2a + 6Q(T), we must require the additional condition that I12aQ(T)I < 1 in order to satisfy eq. (28). This choice, as shown below, leads to a model similar to that proposed by Kobayashi [20].

+ -

specified in terms of w, ( T u - To), and the material parameters. However, the parameters ~" and m are still undetermined because they are related to the unknown quantities 8 and z. We expect the parameter 6 to be much less than w. Hence, we fix the parameter m by conducting an asymptotic analysis of the phase-field equations in the limit ~--->0 with S, a, and m of order one. In this limit, a free boundary problem is recovered. The details are analogous to those given by Caginalp [11] and so for brevity we just give the results. The free boundary problem satisfied by the leading order temperature is

with interfacial boundary conditions

p(~b) = ~b2(3 - 2~b),

Ou ~ Ot

195

(48)

The dimensionless parameters S and a can be

and

[ ou]liquid .U I On d solid

(51)

S '

where [ ' = t r T m / [ W L o ( T M - To) ] is the dimensionless capillary length, 171 is the dimensionless normal velocity of the interface into the liquid and ~ is the dimensionless interracial curvature (measured positive for convex projections into the liquid). The interracial boundary condition eq. (50) reduces to the Gibbs-Thomson equation when tTi = 0. The additional term incorporates the effect of interface kinetics. The dimensionless interface kinetic coefficient is therefore represented by m; it may be related to the corresponding dimensional quantity /z by comparison of eq. (50) with its usual dimensional form: T = TM-

trTM 1 L---"o-~ - --~ v , ,

(52)

which gives m=

/x~rTM xL °

(53)

196

S.-L. Wang et al. / ThermodynamicaUy-consistent

In view of eq. (44), this means that ~- is proportional to 6, which makes m independent of ~" as implied by eq. (41). The only remaining undetermined parameter is therefore ft. In practice, ~" should be chosen small enough to validate the asymptotics but large enough to make computations practical. This completes the determination of the dimensionless phase-field parameters in terms of the physical parameters. The advantages of the phase-field model given by eq. (47) and eq. (48) are two-fold. First, the model is consistent with the ideas of irreversible thermodynamics because it was derived from an entropy functional, which is the appropriate thermodynamic potential in this nonisothermal situation. Second, it is constructed so that the states 4'---0 and 4'--1 correspond to the bulk solid and liquid phases, respectively, independent of the temperature. This has the advantage that latent heat of the correct total amount is liberated only in the interfacial region. The model proposed by Langer [1,2] can be obtained by replacing the term 30g(~b), which appears in both eq. (47) and eq. (48), by unity, which is its average value over the range 0 < 4' < 1, while leaving the term g'(4') in eq. (48) as calculated from eq. (30). This "linearization" would violate eq. (27) and eq. (28). Thus, in the Langer model, the bulk solid and liquid phases do not correspond to constant values of 4' independent of the temperature. In a recent model developed by Caginalp and Chen [13], a function f(4') was introduced in the free energy functional (their equation (1.6)) to identify the bulk phases precisely by 4' = +-1, which is equivalent to maintaining the term 30g(4') in eq. (48), but their model does not have the thermodynamicallyconsistent 30g(4') term in eq. (47).

3.2. Model H Eq. (46) applies, but there is the restriction [12aQ(T)[ < 1. Substituting eq. (46) for p(~b) and eq. (30) for g(4') into eq. (40) and eq. (41) yields the following set of phase-field equations:

phase-field models for solidification

Ou 07

1 [1 - 4'2(3 - 24')] O£(u) s 07

+

4'(1 - 4') o?

= V2u,

(54)

g2,9~ _ ~.z~24' + 4,(1 - 4')[,/, - 1 + 6gaSO.(u)]. mot (55) Recently, Kobayashi [20-23] proposed a phase-field model based on the following pair of dimensionless equations: Ou 1 04' ---: + = V2u Ot S'~-~ ' --2 E 04'

m at

(56)

2

g2f 4' + 4'(1 - 4')(4' - ½ +/3 arctan(vu))

(57) where/3 and v are positive constants with/3 < 1. The phase-field equation in Model II, eq. (55), is identical to that suggested by Kobayashi provided that /3 arctan(vu) Q_(u) = 6~rgaS

(58)

Note that our restriction I12aQ(T)] < 1 is equivalent to Kobayashi's condition/3 < 1. The derivative of the function Q(u) is related to the function L(u) by eq. (43), which gives £(u) = (1 + [(TM - To)/TM]u} 2 1 +

2

'

(59)

and/3 = 6~r~aS/v. The function/~,(u) will have a strong dependence on u unless v is chosen to be very small. This dependence on u requires the heat capacity per unit volume, c s, of the solid to have a definite dependence on temperature, which, from the derivative of the expression es(T) = e L ( T ) - L(T), eq. (31), and eq. (42), is represented by

S.-L. Wang et aL / Thermodynamically-consistent phase-field models for solidification

197

-2 -4 -6 |

- 0 . 075

,

-0.05

,

- 0 . 025

0

O. 025

O. 05

O. 0"75

U

Fig. 2. Plot of the quantity - L ' ( u ) versus u that illustrates (see eq. (60)) the temperature-dependence of the heat capacity per unit volume of the solid, Cs, which is necessary to obtain a thermodynamically-consistent equation for temperature corresponding to Kobayashi's model. The plot is for J, = 10, used by Kobayashi in his computations, and (T u - To)/T ~ = 0.2. For values of the undercooling with S < 1, there will be a rather large variation of c s with temperature, even for temperatures near the melting point.

The quantity -/~'(u) is plotted in fig. 2 for the case ~, = 10 (used by Kobayashi) and ( T M - T o ) / T M = 0.2. We note that the corresponding heat capacity per unit volume will vary considerably, even near the melting point, u = 0, and can possibly become negative. For solidification from a supercooled melt, the temperature in the solid will typically be close to the melting point, with temperature gradients much less than those in the liquid. Nevertheless, there might be problems in using Kobayashi's model for such large values of ~,. Thus, in order to recover the same governing equation for the phase field as Kobayashi, within a thermodynamically-consistent framework, it is necessary for the heat capacity per unit volume of the solid to have the functional dependence on temperature given by eq. (60). However, the self-consistent equation for the temperature will then be eq. (54) instead of Kobayashi's equation (56). We first compare the terms containing 0~b/ 07; they will only be important in the interfacial

region where u ~ 0 so / ~ ( u ) - 1. Thus, replacing 6~k(1- tk) by its average value of 1 over the range 0 < 4) < 1 reproduces Kobayashi's corresponding term. This is similar to the "linearization" required to recover Langer's model from Model I. The term in eq. (54) containing d£/0t', however, is completely absent in Kobayashi's equation (56). It vanishes in the liquid where 4) = 1, but not in the solid where ~b = 0, and arises because of the variable heat capacity per unit volume necessary to make Kobayashi's model thermodynamically consistent. In fact, for ~b = 0, eq. (60) can be used to combine the first two terms on the left-hand side of eq. (54) to yield c s Ou~ C ~t

~2 u

(61)

which is in complete agreement with the classical equation in the solid phase. An alternative approach to comparing our model to that of Kobayashi would be to choose c s and p(~b) to achieve the same equation for the temperature. This would require c s = c and p(~k) = ~b, but then G'(~b) - p'(~b) Q ( T ) = G'(q~)

198

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

- Lo[(1/TM) - ( l / T ) ] , and eq. (27) would require G(0) and G(1) to depend on temperature, which is a contradiction.

4. Discussion

We have employed the method of Penrose and Fife, based on an entropy functional, to derive a class of phase-field models for the crystallization of a pure material from its melt. This method provides a Lyapunov functional [25] which may facilitate the development of numerical solution methods. The parameters of the model are selected by passing to the asymptotic limit of a sharp interface and comparing with the classical model. Criteria are developed to ensure that the phase field will take on fixed values, independent of temperature, for bulk solid and liquid. Specific choices of the phase-field function are made to yield models, which we call Model I and Model II, that bear strong resemblances to the models of Langer and Kobayashi, respectively. However, Models I and II contain nonlinear functions of the phase field that are absent in the models of Langer and Kobayashi, but are necessary to guarantee thermodynamic consistency. Model I differs from Langer's model only in the interfacial region. Model II differs from Kobayashi's model both in the interfacial region and in the bulk solid; in particular, the equation for the temperature that is thermodynamically consistent with Kobayashi's equation for the phase field has a heat capacity per unit volume in the solid phase that is a rather strong function of temperature, even for temperatures close to the melting point. These models also guarantee positive entropy production locally in space. The volumetric entropic production due to heat flow, IqlE/MT, and the entropy flux, q/T, are classical and require no further discussion. The corresponding quantities, ~.(6)2 and ~26V4', require further clarification, which we proceed to give by relating them to analogous quantities for a sharp-interface

model. The volumetric entropy production ~-(6) 2 will contribute only in volume elements do in which ~ differs appreciably from zero. These elements will correspond to regions through which a solid-liquid interface is passing, and for which ~ ~/)1/1~ and d v ~ d a t , where da I is an element of area on the interface. Here we have taken ~7= 6X/2 8 as a more precise representation of the interface thickness; from eq. (35), ~/ represents the distance over which 4' varies from roughly 0.05 to 0.95. Thus, 2

T((~) 2 do ~---rv I d a t = "r/

L0

2

2 vI d a , ,

(62)

/j,T M

where eqs. (44) and (53) have been used. The 2 2 quantity [Lo/(tZTM)]V I turns out to be the entropy production per unit area associated with the movement of a sharp interface for a linear kinetic law of the form represented by eq. (52), as can be shown using the methodology of Gurtin [26]. Similarly, the entropy flux, E2~V4', will only contribute to eq. (6) over area elements da of the control volume through which an interface passes and has a component of its normal growth velocity v I along n. Identifying (~ as above and noting that V4' ~ - v i / ( o i ~ ), we see that E2~V4'

2 Or - - - " ~ - [Ji • n = - - - I)i • n , "0 "0TM

"n~

(63)

where eqs. (36) and (39) have been used to eliminate 6. For an interface corresponding to eq. (35), one can show from eq. (1) that there is no surface excess internal energy per unit area relative to a sharp interface located at x = 0. Therefore, Or=--TM sxs, where s Xs is the surface excess entropy per unit area relative to a sharp interface located at x = 0. Thus we have S xs

¢26V4' • n

da

~ " ~ VI "n d a .

(64)

The area over which this term will contribute to eq. (6) is a thin ribbon defined by the intersection of the diffuse interface with the area M of

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

the control volume. Hence the area element da --~7 csc ~9 d/, where dl is an element of length along the ribbon and O is the angle between v~ and n. This trigonometric factor arises because the diffuse boundary,is not necessarily perpendicular to the surface of the control volume. Thus finally

f

e2~V~b • n da ~ ~sXSvI cot O dl,

(65)

which is in complete agreement with the analysis of Gurtin for a sharp interface model [27,28]. Eq. (65) represents the rate at which entropy exits the control volume by means of the passage of portions of the interface out of the surface of the control volume. It makes no contribution in regions of that surface at which the interface is moving in a direction perpendicular to the normal of the control volume. Penrose and Fife were able to obtain Langer's model from a formalism that guarantees positive entropy production by making the following choices (in our notation, equivalent to their eq. (3.11)):

p(~)=~,

L(T)=Lo,

199

model for the non-isothermal solidification of an alloy. For a binary alloy, for example, it would be necessary to specify the internal energy as a function of T, ~b, and the composition c. This would be a logical extension of the phase-field model for isothermal binary alloy solidification, developed for a lens-type phase diagram in ref. [31]. Another extension is to incorporate arbitrary anisotropy of surface tension and interface kinetics in a thermodynamically-consistent manner [32].

Acknowledgements The authors are grateful for discussions with W.J. Boettinger. This work was performed with support from a NATO collaborative grant, the Applied and Computational Mathematics Program of DARPA, the Microgravity Science and Applications Program of NASA, and the National Science Foundation, under grant DMR9211276. One of the authors (R.J.B.) was supported by a National Research Council Postdoctoral Fellowship.

es(T)=A-B/T,

where A and B are constants. This choice of p(~b), in view of eq. (27), would require G(~b) to depend on T, a contradiction. Therefore, for their model, the values of 4' corresponding to the bulk phases will depend on temperature. Recently we became aware of work by Umantsev and Roitburd [29] and by Umantsev [30] on a phase-field model that has many features similar to ours, including fixed values of the phase field in the bulk phases. Umantsev's model is based on a Ginzburg-Landau functional that is the integral of a Gibbs free energy per unit volume and a gradient energy. Some aspects of their results could be obtained by adding a gradient energy contribution to our internal energy functional, eq. (1). The methodology developed in the present paper can be extended to develop a phase-field

References [1] J.S. Langer, private communication (August 1978). [2] J.S. Langer, in: Directions in Condensed Matter Physics, eds. G. Grinstein and G. Mazenko (World Scientific, Singapore, 1986) p. 165. [3] B.I. Halperin, P.C. Hohenberg and S.-K. Ma, Phys. Rev. B 10 (1974) 139. [4] J.B. Collins and H. Levine, Phys. Rev. B 31 (1985) 6119. [5] G. Caginalp, in: Applications of Field Theory to Statistical Mechanics, ed. L. Garrido, Lecture Notes in Physics, Vol. 216 (Springer, Berlin, 1985) p. 216. [6] G. Caginalp, in: Material Instabilities in Continuum Problems and Related Mathematical Problems, ed. J.M. Ball (Oxford Univ. Press, Oxford, 1988) p. 35. [7] G. Caginalp and EC. Fife, Phys. Rev. B 33 (1986) 7792. [8] G. Caginalp, Arch. Rat. Mech. Anal. 92 (1986) 205. [9] G. Caginalp, Ann. Physics (NY) 172 (1986) 136. [10] G. Caginalp and P.C. Fife, SIAM J. Appl. Math. 48 (1988) 506. [11] G. Caginalp, Phys. Rev. A 39 (1989) 5887.

200

S.-L. Wang et al. / Thermodynamically-consistent phase-field models for solidification

[12] G. Caginalp and E.A. Socolovsky, J. Comp. Phys. 95 (1991) 85. [13] G. Caginalp and X. Chen, in: On the Evolution of Phase Boundaries, eds. M.E. Gurtin and G.B. McFadden, The IMAVolumes in Mathematics and Its Applications, Vol. 43 (Springer, Berlin, 1992) p. 1. [14] M.E. Gurtin, in: Metastability and Incompletely Posed Problems, eds. S. Antman, J.L. Ericksen, D. Kinderlehrer and I. Muller, The IMA Volumes in Mathematics and Its Applications, Vol. 3 (Springer, Berlin, 1987) p. 135. [15] P.C. Fife and G.S. Gill, Physica D 35 (1989) 267. [16] P.C. Fife and G.S. Gill, Phys. Rev. A 43 (1991) 843. [17] G.J. Fix, in: Free Boundary Problems: Theory and Applications, Vol. II, eds. A. Fasano and M. Primicerio (Pitman, Boston, 1983) p. 580. [18] J.-T. Lin, The Numerical Analysis of a Phase Field Model in Moving Boundary Problems, Doctoral Thesis, Department of Mathematics, Carnegie Mellon University (1984). [19] S.A. Schofield and D.W. Oxtoby, J. Chem. Phys. 94 (1991) 2176. [20] R. Kobayashi, Bull. Jpn. Soc. Ind. Appl. Math. 1 (1991) 22.

[21] R. Kobayashi, in: Computing Optimal Geometries, Proc. AMS Special Session, ed. Jean Taylor, videotapes (1991). [22] R. Kobayashi, Physica D 63 (1993) 410. [23] R. Kobayashi, in: Pattern Formation in Complex Dissipative Systems, ed. S. Kai (World Scientific, Singapore, 1992) p. 121-128, and associated video tape. [24] A.A. Wheeler, B.T. Murray and R.J. Schaefer, Physica D 66 (1993) 243. [25] O. Penrose and P.C. Fife, Physica D 43 (1990) 44. [26] M.E. Gurtin, Arch. Rat. Mech. Anal. 104 (1988) 195. [27] M.E. Gurtin, Arch. Rat. Mech. Anal. 96 (1986) 199. [28] M.E. Gurtin, in: PDE's and Continuum Models of Phase Transitions, eds. M. Rascle, D. Serre and M. Slemrod, Lecture Notes in Physics, Voi. 344 (Springer, Berlin, 1989) p. 99. [29] A.R. Umantsev and A.L. Roitburd, Sov. Phys. Sol. State 30 (1988) 651. [30] A. Umantsev, J. Chem. Phys. 96 (1992) 605. [31] A.A. Wheeler, W.J. Boettinger and G.B. McFadden, Phys. Rev. A 45 (1992) 7424. [32] G.B. McFadden, A.A. Wheeler, R.J. Braun, S.R. Coriell and R.F. Sekerka, Phase-field models for anisotropic interfaces, Phys. Rev. E 48 (1993), in press.